api 572 study guide
Embed Size (px)
API 572 Study GuidePractice QuestionsThis following is a study aid that you can use to learn the details and content of API RP-572, Inspection of Pressure Vessels. There will be about 15-25 questions from this document on the API 510 exam. We do not spend time in class discussing this publication. So it is important that you become familiar with this content in your personal study sessions. Note! The study guide does not at this time have any questions for API 572 Appendix A. There will be some questions from Appendix A on the API exam. The questions in this study aid are in the same order as API 572. An answer key will be provided in class. Its helpful to read a few pages of API 572 and then answer the questions associated with these pages. We suggest that you do this study guide at least twice prior to the API exam.
Most pressure vessels are subjected to internal or external pressure that exceeds: a) b) c) d) 5 psig. 15 psig. 25 psig. 50 psig.
External pressure is usually caused by a vacuum or by using a ____________________ vessel. Vessel shell rings are normally made by: a) b) c) d) e) rolling plate at ambient temperatures. rolling plate at elevated temperatures. rolling plate at either elevated or ambient temperatures. forging. casting and machining.
Shells constructed with multi-layers (a number of thin cylindrical sections) are normally used for vessels having: a) b) c) d) high design temperatures. high design pressures. exotic materials. a small diameter.
Match the material with the service: A. B. C. Carbon Steel Copper Alloys Titanium _________ _________ _________ Cooling Water Sea Water Most Common Material
What is the primary purpose for installing a lining on the inside of a vessel? a) b) c) d) Resist corrosion Improve heat transfer Improve fluid flow by decreasing the friction inside the vessel Minimized effort to clean vessel at future turnarounds
When is a pressure vessel shell normally made from an alloy material? a) b) c) d) Corrosive service High operating pressures High operating temperatures Either high operating pressure or high operating temperature
API 572 Study GuidePractice Questions8. List four types of Metallic Liners. a) b) 9. _________________________________ _________________________________ c) _________________________________ d) _________________________________
What are the two primary purposes for non-metallic liners? a) b) c) d) e) Resist erosion, insulate to reduce shell temperature Insulate to reduce shell temperature, resist thermal expansion Resist corrosion, resist thermal expansion Resist stress corrosion cracking, insulate to reduce shell temperature Beautify the facility, improve rate of heat transfer
What is the most common feature of vessels that operate with a vacuum? a) b) c) d) Internally braces Stiffening rings Refractory lining Hemispherical heads
An optionally part of an exchanger that is used to protect the tubes at the inlet nozzle is called a(n): a) b) c) d) baffle. demister mat. impingement plate. strip lining.
What code is often used when constructing vessels that operate at high pressures? a) b) c) d) ASME B&PV Code Section VIII Division 1. ASME B&PV Code Section VIII Division 2 API/ASME Vessel Code. TEMA
What codes are used when constructing a heat exchanger that is used in the petrochemical industry? a) b) c) d) API 660, ASME Section VIII, TEMA API 661, ASME Section VIII, TEMA API 660, API 661, TEMA API 660, API 661,. ASME Section VIII,
All vessel manufacturers that build vessels to ASME Section VIII must have: a) b) c) d) an API 510 inspector on staff. access to an AWS inspector. a written quality-control manual. a machine capable of making dished heads.
The vessel manufacturer stamps the vessel with the code symbol U. What is the meaning of a this code stamp? a) b) c) d) e) All applicable requirements of the ASME Code have been met All requirements of the U-Section in the ASME Code have been met Vessel has been hydrotested Vessel has been radiographed Vessel wall is of uniform thickness
API 572 Study GuidePractice Questions16. A vessel should be maintained in accordance with the: a) b) c) d) 17. 18. construction code. latest edition of ASME Section VIII. code that was last used to rate the vessel. pre-2000 edition of ASME Section VIII.
An inspector should be familiar with any _____________________ that govern the inspection and maintenance of pressure vessels. List the 2 basic reasons for inspection of pressure vessels 1) 2) ________________________________________________________________ ________________________________________________________________
List the 3 basic forms of deterioration 1) 2) 3) ______________________________________________ ______________________________________________ ______________________________________________
The corrosion rate resulting from corrosion-erosion is often: a) b) c) d) higher than the corrosion rate from corrosion without erosion. lower than the corrosion rate from corrosion without erosion. higher in stagnant areas. uniform throughout the whole vessel.
List process conditions that that could change the corrosion rate. 1) 2) 3) 4) 5) ______________________________________________ ______________________________________________ ______________________________________________ ______________________________________________ ______________________________________________
What metallurgies are most affected by CUI? a) b) c) d) Carbon steel and low chromes Carbon steel and all chromes Carbon steel and stainless steels Carbon steel, chromes and stainless steels
List the temperature range where CUI is most prevalent: 1) 2) Carbon Steels Stainless Steels _________________oF _________________oF
Insulated carbon steel vessels may be subject to CUI if operating: a) b) c) d) above the lower-transformation temperature. below the upper transformation. in an intermittent service. above 700 oF. 3 September 2005
API 572 Study GuidePractice Questions25. Which of the following methods is NOT used to detect CUI? a) b) c) d) e) 26. Weld quality RT Profile RT Guided-wave UT Electromagnetic methods Visual inspection after removal of insulation
Which deterioration mechanism can cause direction grooving? a) b) c) d) Erosion Oxidation Sulfidation Temper-embrittlement
List four common areas where corrosion-erosion can occur. 1) 2) 3) 4) ______________________________________________ ______________________________________________ ______________________________________________ ______________________________________________
Match up the corrosion mechanism with the applicable material. (SCC = stress corrosion cracking) A) B) C) D) E) Chloride SCC Polythionic SCC Caustic SCC Amine SCC Carbonate SCC _____ Alkaline systems _____ Non-stress relieved carbon steel _____ Stainless steel _____ Operating temperatures over 400 oF _____ Sensitized stainless steel
When checking for cracks, which of the following inspection techniques is useful only for surface or near-surface cracks? a) b) c) d) Acoustic emission Eddy current Radiography UT angle beam
What is a useful technique to use to evaluate the vessel cladding from outside surface of the vessel? a) b) c) d) Acoustic emission Eddy current Profile radiography UT thickness gauging
During an internal inspection, operating deposits are found in a specific section of the vessel. The inspector must: a) b) c) d) have all deposits removed. determine the cause of the deposits. determine if corrosion is occurring under the deposits. record the volume of the deposits.
API 572 Study GuidePractice Questions32. Which deterioration mechanism is caused by cyclic stresses? a) b) c) d) 33. Creep Fatigue Graphitization Temper-embrittlement
Which of the following vessels is most susceptible to fatigue? a) b) c) d) Coke drum Crude column FCCU regenerator Hydrotreater reactor
What is a common cause for high-cycle fatigue? a) b) c) d) Low operating temperatures High operating temperatures High operating pressures Excess vibrations from mechanical equipment
Cracking occurring in deaerators is attributed to: a) b) c) d) corrosion fatigue. mechanical fatigue. thermal fatigue. velocity fatigue.
A prime location for thermal fatigue is at: a) b) c) d) circumferential welds. dissimilar welds. stainless steel welds. chrome welds.
What NDE method checks for cracks by increasing the vessel pressure above its normal operating pressure? a) b) c) d) Acoustic emission Eddy current Guided wave UT MFL
Why is it difficult to find fatigue cracking? a) b) c) d) Fatigues cracks are very tight It is very difficult to predict the location of fatigue cracking The growth rate of fatigue cracks is very slow It takes many cycles to initate the crack, but relatively few cycles to propagate the crack all the way through the vessel wall.
List the three primary factors of creep: 1) 2) 3) __________________________ __________________________ __________________________ 5 September 2005
API 572 Study GuidePractice Questions40. 41. Creep cracking begins to occur in 1- chrome steels at temperatures above __________ oF. At high temperatures: a) b) c) d) 42. atomic hydrogen reacts to form water. atomic hydrogen reacts to form hydrocarbons. molecular hydrogen disassociates to form atomic hydrogen. molecular hydrogen disassociates to form water.
Which of the following can permeate steel (migrate through the steel)? a) b) c) d) Atomic hydrogen Atomic hydrogen and molecular hydrogen Atomic hydrogen and atomic helium Molecular hydrogen and helium
Susceptibility to HTHA attack increases as: a) b) c) d) chrome content increases. nickel content increases. metal grain size decreases. metal grain size increases.
Susceptibility to HTHA attack increases as: a) b) c) d) operating temperature decreases. operating pressure decreases. carbon content increases. molybdenum content increases.
HTHA can occur in 1- chrome steels at temperatures above __________ oF. What publication provides safe operation limits for steels operating in hydrogen service? a) b) c) d) e) ASME Section II ASME Section VIII API 579 API 941 API 2201
High temperature sulfidation can begin to occur at temperatures above __________ oF. High temperature sulfide attack usually appears as: a) b) c) d) cracks. localized thinned areas. pits. uniform corrosion.
A partial buried vessel should be inspected for soil-to-air corrosion. To perform this inspection, the soil should be excavated: a) b) c) d) 1 to 2 inches. 3 to 6 inches. 6 to 12 inches. 12 to 36 inches.
API 572 Study GuidePractice Questions50. Small living organisms are the cause of biological corrosion. There are various ways that these living organisms cause the actual corrosion to occur. Which of the following is NOT a way biological corrosion occurs? a) b) c) d) 51. Hydrogen normally slows down the corrosion rate on the external surface. Organisms consumes (reacts with) hydrogen. Since less hydrogen is now available, the corrosion rate to increase. Creates an electrolytic concentration cell Creates by-products that are corrosive Creates atomic nitrogen. Atomic nitrogen reacts with iron to form iron nitrate.
What is a common micro-organism in soils that can cause biological corrosion? a) b) c) d) amoebas chloride-reducing bacteria sulfate-reducing bacteria oxygen-reducing parasites
Changes in a metals microstructure can be caused by: a) b) c) d) improper heating and cooling. excessive thermal expansion. operating at cold temperatures. pressure cycles.
Match up the deterioration mechanism with the applicable description. A) B) C) D) Decarburization Graphitization Dealloying Temper Embrittlement _____ Selective leaching of a material in an alloy _____ Loss of carbon near surface of ferrous material _____ A metallurgical change that occurs to Cr-Mo alloys due to operating at high temperatures _____ Conversion of carbides to carbon nodules
What two factors cause decarburization in ferrous materials? a) b) c) d) Low operating temperatures, and numerous pressure cycles High operating temperature, and numerous pressure cycles Low operating temperatures, and a process that reacts with carbon High operating temperature, and a process that reacts with carbon
Which of the following is NOT a problem caused by decarburization? a) b) c) d) Material strength decreases Material toughness decreases Hardness of material increases Fatigue strength decreases
Decarburization is found using: a) b) c) d) metallography. straight beam UT. penetrant testing. MFL.
API 572 Study GuidePractice Questions57. What materials are most susceptible to Graphitization? a) b) c) d) e) 58. Carbon steel and carbon molybdenum steel Carbon steel and low chromes (through 5% chrome) Carbon steel and all chromes High nickel alloys Stainless steels
Graphitization occurs when a susceptible material is subject to: a) b) c) d) many temperature cycles. a prolonged exposure to temperatures above 450oF. a prolonged exposure to temperatures above 825oF. atomic hydrogen.
Which type of graphitization is most likely to lead to a mechanical failure? a) b) c) d) Localized graphitization Random graphitization Uniform graphitization Spot graphitization
In some water services, dezincification can occur in which materials? a) b) c) d) Brass Bronze Monel Alloy 20
What materials are most susceptible to temper embrittlement? a) b) c) d) e) Carbon steel and carbon molybdenum steel Carbon steel and low chromes (through 5% chrome) Low chromes All chromes Stainless steels
Temper embrittlement is caused when a susceptible material is subject to: a) b) c) d) low temperatures. a prolonged exposure to temperatures above 750oF. a prolonged exposure to temperatures above 1100oF. atomic hydrogen.
Brittle fracture is usually not a concern when using: a) b) c) d) carbon steels. low chromes. thin-wall materials. post-weld heat treat materials.
When do most brittle failures in pressure vessels occur? a) b) c) d) During the vessels first winter weather During the first hydrotest After prolong exposure to temperatures above 250oF. After the first pressure cycle 8 September 2005
API 572 Study GuidePractice Questions65. Brittle failures initiate at a notch or stress concentration. Most often, this the initiating point is a: a) b) c) d) 66. tee joint or angle joint, e.g. nozzle-to-shell weld, tray ring weld. stamping in the vessel component. lamination in the plate. welding flaw.
Which of the following deterioration mechanisms can be corrected by annealing the steel? a) b) c) d) Decarburization Dealloying Temper embrittlement HTHA
The most common method to check for freeze damage is by: a) b) c) d) visual inspection. eddy current examination. digital UT. angle beam UT.
Hydriding of titanium alloys is caused when the material absorbs: a) b) c) d) hydrogen. oxygen. nitrogen. zinc.
Which of the following is NOT a potential result of an improper heat treatment? a) b) c) d) e) f) g) High residual stresses Increased density of material Hard zones in material Soft zones in materials Increased material strength Decreased material strength Increased susceptibility to cracking
When setting the inspection interval for the internal inspection, an interval is selected so that at the next inspection: a) b) c) d) the wall thickness is not less than the minimum required thickness. at least 0.100 of corrosion allowance remains. at least 25% of the current corrosion allowance should still remain. at least 50% of the current corrosion allowance should still remain.
One important factor in developing an inspection plan for the next inspection is to occasionally check the: a) b) c) d) Operating departments equipment records. Maintenance departments equipment records. Financial departments equipment records. Environmental departments equipment records.
API 572 Study GuidePractice Questions72. Before performing a vessel inspection, which of the following activities does the inspector NOT need to do? a) b) c) d) e) 73. Review past inspection records. Check with Operations to determine whether there were any abnormal operating conditions. Review the equipment construction details. Review the vessels service conditions Determine what is being offered as the daily special at the local lunch caf.
A vessel has a refractory lining. During the internal inspection, an small area of damaged refractory is found. It is now important to: a) b) c) d) replace the refractory with superior materials. remove enough of the refractory to determine the condition of the base metal. remove the damaged refractory plus 50% more to determine the base metal condition. remove and replace all the refractory in the entire vessel.
All NDE tools should be: a) b) c) d) calibrated daily. calibrated weekly. rated for the appropriate gaseous atmosphere. certified by UL-142.
When performing a PT examination inside an exchanger shell, what is one potential problem? a) b) c) d) Residual penetrant can cause crevice corrosion Residual penetrant can cause steel to become anodic Vapors from the exam can displace air It is more difficult to prepare the shell for the exam as compared to other NDE methods
Ladders and platforms should be inspected: a) b) c) d) only with a visual examination. by visual examination and UT. by visual examination and RT. by visual examination and hammer-testing.
Small depressions on platforms are of concern since these can: a) b) c) d) collect and hold water, potentially causing accelerated corrosion. create a tripping hazard. create flexing that could cause a fatigue failure. be rather ugly and prevent your facility from achieving APIs Petrochemical Facility of the Year award.
Crevice corrosion is NOT common at which of the following locations? a) b) c) d) Under nuts on anchor bolts At repad-to-shell welds Where handrail supports slip into platform sleeves Between exchanger shell and cradle support
API 572 Study GuidePractice Questions79. Which of the following is usually NOT a cause of large cracks in a concrete foundations? a) b) c) d) 80. High temperature. Excessive settlement. Poor design. Poor materials.
Small hair-like cracks in concrete foundations: a) b) c) d) should always be caulked. should always be repaired with a cement material similar to the original material. should be further examined by hammer-testing. are usually not a serious concern.
A distorted anchor bolt is usually the result of: a) b) c) d) serious foundation settlement. selecting the wrong material for the anchor bolt. using an anchor bolt of insufficient diameter. using an anchor bolt of insufficient length.
What examination method is normally used to examine in-service anchor bolts? a) b) c) d) e) Visual UT Eddy current Hammer-testing Acid etching
What is the best way to prevent external corrosion on structural steel? a) b) c) d) Painting Fireproofing Galvanizing Insulation
What is a good way to check for disbanded fireproofing? a) b) c) d) e) Visual examination UT Eddy current Hammer-testing with light taps Sledge hammer-testing with a 25 lb sledge hammer
What is one important item to check during an External inspection of an exchanger? a) b) c) d) Surface temperature at the inlet and outlets The floating end of the exchanger is free to slide on its support Determine the fluid flow rate through both the shell side and tube side of the exchanger Measure the clearance between the shell and the ground
Guy wires supporting tall vessels should be examined using: a) b) c) d) visual examination. UT. profile RT. acoustic emission. 11 September 2005
API 572 Study GuidePractice Questions87. Guy wire clips should be placed at a spacing of at least: a) b) c) d) 88. 3. 6. 3 guy wire diameters. 6 guy wire diameters.
Which of the following would be most affected if a vessel foundation experiences excessive settlement? a) b) c) d) e) Stiffener rings Relief devices Nozzles with attached piping Manways Top head
What should be done if shell distortion is found at a nozzle? a) b) c) d) Check for cracking on all nozzle welds Check the hardness of nozzle welds and nozzle components Check thickness by taking UT readings on a 2 grid on all nozzle components and on the distorted area of the shell. Only note the distortion in your inspection report
90. 91. 92.
Catalytic reformer vessels may have creep damage if the operating temperature is above _______ oF The grooves on an existing ring-joint flange should be checked for ___________________. Grooves on existing stainless steel flanges should be checked for: a) b) c) d) stress corrosion cracking. temper embrittlement. dealloying. corrosion fatigue.
Existing slip-on flanges should be checked for: a) b) c) d) chloride cracking. creep. crevice corrosion. graphitization.
Vessel grounding connections are primarily needed to provide a path for electrical current from: a) b) c) d) a lighting strike or from a welding machine. a lighting strike or from static electricity. a welding machine or from an electrical short. an electrical short or from static electricity.
The maximum permitted resistance-to-ground for a vessel grounding system is: a) b) c) d) e) 0.5 ohms. 5.0 ohms. 10 ohms. 25 ohms. 50 ohms.
API 572 Study GuidePractice Questions96. Which of the following coating failures is easily missed during a visual examination? a) b) c) 97. Film lifting Blisters Rust spots
Where are two likely areas where paint failures occur? a) b) c) d) e) Top heads and nozzles Weld seams and nozzles Top heads and moist crevices Weld seams and moist crevices Nozzles and moist crevices
What two on-stream NDE techniques may be able to locate moist insulation? a) b) c) d) e) f) Real-time RT and Thermography Real-time RT and MFL Neutron back scatter and Thermography Neutron back scatter and MFL Neutron back scatter and Real-time RT Thermography and MFL
99. 100. 101.
Pit depth is normally measured with a ________________________________. The minimum number of TMLs required for a routine vessel is at least _______ thickness reading(s) on each shell ring, and _______ thickness reading(s) on each head. A vessel operates in a cyclic temperature service. The vessel support-to-vessel welds should be checked using MT or PT to check for: a) b) c) d) stress corrosion cracking. fatigue cracking. polytheonic cracking. HTHA.
Which of the following is NOT a significant factor in atmosphere corrosion? a) b) c) d) vessel operating pressure relative humidity chemical vapors metal surface temperature
In a caustic storage vessel, caustic embrittlement is least likely at: a) b) c) d) heating coil connections. areas of high stress. internal baffles or vortex breakers. nozzles.
Caustic that seeps through a crack will often leave a: a) b) c) d) brown residue. white salt. yellow sticky deposit. black hard residue.
API 572 Study GuidePractice Questions105. A vessel contains an acid corrodent. The areas directly below the liquid level are likely to be subject to: a) b) c) d) e) 106. hydrogen blistering. HTHA. temper embrittlement. graphitization. caustic cracking.
Blisters on a vessel shell can be easily detected with: a) b) c) d) UT. RT. visual exam using a flashlight beam perpendicular to the shell. visual exam using a flashlight beam parallel to the shell.
Small blisters can be easily detected by: a) b) c) d) feeling the surface with your fingers. hammer testing. MT or PT. magnetic flux leakage.
Why is wet fluorescent magnetic particle testing often used to detect certain types of cracking? a) b) c) d) Easier to perform than other types of MT Requires less effort to qualify the NDE examiner as compared to dry MT More sensitive technique as compared to dry MT Equipment to perform the exam is less expensive than what is needed for other MT exams
Tough question! The temperature of a hot-spot on a refractory lined vessel should be periodically checked. Which of the following is NOT an acceptable method for checking the temperature? a) b) c) d) Portable thermocouple Thermography Temperature indicating crayons. Place your hand on surface for exactly 1 second. Calculate the vessel temperature based on the depth of the 3rd degree burns on your hand.
A hot-spot has developed on a refractory lined carbon steel vessel. During the next internal inspection the wall at the hot-spot should be metallurgically examined whenever the metal temperature has exceeded: a) b) c) d) 450 oF. 750 oF. 850 oF. 1100 oF.
Normal vessel cleaning methods, like steam cleaning, usually are adequate to meet the inspectors needs for an internal inspection. Extra cleaning such as abrasive-grit or water blasting may be required when inspecting for: a) b) c) d) localized thin areas. deep pitting. stress corrosion cracking. thermal fatigue cracking.
API 572 Study GuidePractice Questions112. An internal inspection will be performed on a vessel. What is the initial step to be performed? a) b) c) d) 113. Collect all necessary inspection tools Check the vessel permitting requirements Collect the necessary personnel protective equipment Read the previous inspection reports
Sulfidation is a common concern at the: a) b) c) d) top of the crude units fractionating column. bottom of the crude units fractionating column. top of a hydrotreater reactor. bottom of a hydrotreater reactor.
A vessel subject to wet hydrogen sulfide or cyanide environments is susceptible to. a) b) c) d) cracks in the base metal. cracks in the weld and heat affected zones. localized thin areas (LTAs). extensive pitting.
If sludge settles on the bottom head of a vessel, what corrosion mechanism is likely to occur? a) b) c) d) Stress corrosion cracking Dealloying Concentration cell corrosion Sludgitization
If steam is injected into a vessel, a likely place for corrosion is on the: a) b) c) d) inlet nozzle. vessel wall opposite the nozzle. vessel wall directly below the nozzle. vessels anchor bolts. (once again proving it is difficult to come up with 3 wrong answers!)
When a reboiler is used with a tower (fractionating column), a common place for corrosion is: a) b) c) d) the inlet to the reboiler. top head of the tower. at the tower where the hot process returns. at the tower where the cold process returns.
What is the normal cause of corrosion associated with reboilers? a) b) c) d) Hot process decomposes to form acids Hot process decomposes to form polytheonic caustic Increased velocity of returning process causes erosion Deposits in the process cause oxygen pitting
Most cracks that occur in a vessel occur at ______________________. Exchangers in cooling water service have the highest corrosion rates where the: a) b) c) d) velocity is the highest. velocity is the lowest. ph is the highest. water temperature is the highest. 15 September 2005
API 572 Study GuidePractice Questions121. An impingement plate is installed on an exchanger bundle. What area is most susceptible to corrosion? a) b) c) d) 122. Exchanger shell near the impingement plate Tubesheet Tubes near the impingement plate Inlet nozzle
During an internal inspection: a) b) c) d) at least 10% of all welds should be checked with either MT or PT. 100% of the internal surface should be cleaned. thickness readings should be taken at suspect locations. hammer-testing should be performed on all nozzles.
List 4 major areas where cracks occur in vessels made of low chromes (i.e. 1-1/4 & 2-1/4 Cr). a) b) c) d) __________________________________________ __________________________________________ __________________________________________ __________________________________________
A very effective means to find cracks is by using: a) b) c) d) MFL. red dye PT. dry particle MT. wet fluorescent particle MT.
Which of the following steels is most likely to crack? a) b) c) d) Steels with a tensile strength lower than 70,000 psi Steels with a yield strength above 20,000 psi. Coarse-grain steels Fine-grain steels
Normally tower (column) trays are inspected using: a) b) c) d) only a visual examination. visual examination and UT. visual examination and some type of crack detection NDE method. visual examination, UT and some type of crack detection NDE method.
Often corrosion will occur on the shell of an exchanger at the location of the baffles. An easy way to find this corrosion is by: a) b) c) d) spot UT. visual examination. eddy current testing. shining a flashlight beam parallel to the shell.
API 572 Study GuidePractice Questions128. Areas directly above the liquid level in vessels containing acidic corrodents s are subject to: a) b) c) d) e) f) 129. caustic embrittlement. hydrogen blistering. graphitization. creep. fatigue. dealloying.
How can small blisters easily be found? a) b) c) d) Feel metal surface with your fingers Visual examination Hammer-testing Spot UT readings
Existing exchanger shells sometimes become out of round making it difficult to reinsert the bundle. What is the most common cause of exchanger shell out-of-roundness? a) b) c) d) e) f) Over pressure Elevated temperature Metal fatigue Creep Welding repairs to the shell Meteor strike
Vessels containing amines are subject to: a) b) c) d) e) oxygen pitting. oxidation. cracking. caustic embrittlement. dew point corrosion.
Deaerators used for boiler feedwater are subject to: a) b) c) d) e) pitting. localized thinned areas. uniform corrosion. cracking. dealloying.
Loose or cracked metallic linings can be found using: a) b) c) d) light taps with a hammer. visual inspection. MT. acoustic emission.
Bulged linings are often the indication of a _______________ in the liner. Whenever there are indications that a metallic liner has leaked, it is important to determine the: a) b) c) d) thickness of the liner. displacement of the bulged area. condition of the base metal under the liner. the identification of the welder who previously installed the liner. 17 September 2005
API 572 Study GuidePractice Questions136. What type of weld metal overlay is often used for hydrotreater reactors? a) b) c) d) e) 137. Low chromes High chromes Austenitic stainless steel Stabilized austenitic stainless steel High nickel alloys
What are the two primary purposes for refractory linings? 1) 2) ____________________________________________ ____________________________________________
A break or void in a paint coating is called a: a) b) c) d) e) blister. film lift off. holiday. voidea. lamination.
A common tool used to find breaks in a pipe coating is: a) b) c) d) acoustic emission. eddy current. MFL (magnetic flux leakage). spark testing.
Spark testing is being performed on a coating. What happens if the voltage on a spark tester exceeds the dielectric strength of the coating? a) b) c) d) e) Coating will become magnetic Strength of the coating bond increases A hole is blown in the coating Coating will crack Creates a nuclear chain reaction that will destroy the entire universe
A common tool used to inspect refractory is a _________________________. Extra metal thickness in a vessel is: a) b) c) d) sometimes used as nozzle reinforcement. always considered extra corrosion allowance. always clearly identified on a U-1 form. never allowed.
When a refractory lining cracks, what is a common problem that occurs to the base metal? a) b) c) d) Dew point corrosion Dealloying Excessive thermal stress Brittle failure
API 572 Study GuidePractice Questions144. What method is often used to detect metallurgical changes to the base metal? a) b) c) d) e) 145. Tension tests Bend tests Metallography Flash radiography Impact tests
What method is often used to detect carburization and decarburization? a) b) c) d) e) Tension tests Bend tests Metallography Hardness testing Impact tests
It is recommended NOT to hammer test vessels that are _________________________. Which of the following is NOT a purpose of a pressure test? a) b) c) d) Validate vessel MDMT Assure equipment tightness Assure equipment integrity Redistribute stresses at discontinuities
What is the most important concern when hydrotesting a large in-service vessel? a) b) c) d) Rope off an area equal to 1000 sq. ft. for every 1 of vessel height Provide multiple calibrated pressure gauges Assure the water used has less than 50 ppm of particulates Assure vessel foundation and supports are adequate for the hydrotest weight
Acoustic emission testing is especially useful on: a) b) c) d) vessels of simplistic design. vessels where internal inspections are difficult to perform. large vessels. heat exchangers.
A pneumatic pressure test is performed on a large vessel. What is one way to determine the location of remote leaks? a) b) c) d) Block-in the vessel and see if the pressure drops UT leak detector Binoculars Thermography
A vessel is being vacuum tested. What is one negative aspect of a vacuum test? a) b) c) d) Location of leak is not easily identified There are additional safety precautions as compared to a hydrotest Creating the vacuum requires expensive equipment The vacuum must be held for 24 hours
API 572 Study GuidePractice Questions152. An in-service vessel has a shell thickness of 2.5. The minimum metal temperature allowed during a pressure test is: a) b) c) d) e) 153. 10oF. 30oF. 60oF. 10oF. above the vessel MDMT. 30oF. above the vessel MDMT.
An in-service vessel has a shell thickness of 1.25. The minimum metal temperature allowed during a pressure test is: a) b) c) d) e) 10oF. 30oF. 60oF. 10oF. above the vessel MDMT. 30oF. above the vessel MDMT.
When performing a pneumatic pressure test, the requirements of which code should be followed? a) b) c) d) e) f) ASME B&PV Section I ASME B&PV Section V ASME B&PV Section VIII ASME B31.3 API 579 API 2201
A shell-side pressure test is being performed on an exchanger with a floating head bundle. The bundle is in the shell and the channel cover is removed. This test will show overall bundle integrity and can be used to specifically locate which of the following leaks? a) b) c) d) e) Stationary tubesheet roll leaks Floating head tubesheet roll leaks Floating head gasket leak. Leaking tubes The exact location of any leak cannot be determined with this test
A tube-side pressure test is being performed on an exchanger with a floating head bundle. The bundle is in the shell and the piping connected to a bottom shell nozzle is removed. This test will show overall bundle integrity and can be used to specifically locate which of the following leaks? a) b) c) d) e) Stationary tubesheet roll leaks Floating head tubesheet roll leaks Floating head gasket leak. Leaking tubes The exact location of any leak cannot be determined with this test
A tube-side pressure test is being performed on an exchanger with a floating head bundle. The bundle is outside the shell and a test head is bolted to the stationary tubesheet. This test will show overall bundle integrity and can be used to specifically locate which of the following leaks? a) b) c) d) e) f) Stationary tubesheet roll leaks Floating head tubesheet roll leaks Floating head gasket leak. Leaking tubes Roll leaks on both ends, tube leaks, and floating head gasket leaks The exact location of any leak cannot be determined with this test 20 September 2005
API 572 Study GuidePractice Questions158. During a bundle pressure test, a leaking tube is discovered. The inspection results indicate that the other tubes are acceptable for a future operational run. The leaking tube is normally: a) b) c) d) e) 159. replaced in kind. replaced with improved metallurgy. plugged. removed. rerolled.
During a bundle pressure test, a tube roll-leak is discovered. The inspection results indicate that the other tubes are acceptable for a future operational run. The leaking tube is normally: a) b) c) d) e) replaced in kind. replaced with improved metallurgy. plugged. removed. rerolled.
Before applying a hydrotest to the shell-side of a carbon steel bundle, it is important to: a) b) c) d) determine whether the tubes are thick enough for the external pressure. determine how far an area should be roped off.. assure that all tubes have been seal-welded at the tubesheet. check the chloride content of the water.
Before applying a high-pressure hydrotest to a bundle, it is important to: a) b) c) d) connect a PRV to prevent excessive pressure. have multiple pressure gauges connected for the test. assure that all tubes have been seal-welded at the tubesheet. determine whether the tubesheet is thick enough for the pressure.
A shell has a minimum thickness of 0.352 and has a corrosion allowance of 0.125. The total thickness needed is 0.477, so the designer orders 0.500 plate. The extra 0.023 is usually consider extra corrosion, but often the designer uses the extra metal (and the extra is no longer extra): a) b) c) d) in the design of vessel stiffening. in the design of nozzle reinforcement. to improve the joint efficiency. to minimize the number of RTs..
Which of the following components usually does NOT have a specified minimum thickness? a) b) c) d) e) Top head Nozzle reinforcement Metallic liner Platform handrail Internal baffle
If a jurisdiction requires a vessel repair to meet the National Board Inspection Code, what stamp would have to be used by the Repair Organization? a) b) c) d) e) A U UV R VR 21 September 2005
API 572 Study GuidePractice Questions165. A corroded shell area that has an area of 2.5 ft2 is built-up with weld metal. How should the repair area normally be inspected? a) b) c) d) 166. Visual examination Visual examination and either MT or PT Visual examination and spot UT Visual examination and eddy current
When removing a crack in a vessel using flame or arc gouging: a) b) c) d) care must be taken to prevent the crack from growing. the craftsman must be qualified in accordance with ASME B&PV Section IX. the base metal should only be a P1 or P-3 material. the crack length cannot be greater than allowed in API 579.
A crack in a vessel is removed. The groove: a) b) c) d) e) must always be filled with weld metal of the same metallurgy as the base metal. should be filled with weld metal of a higher alloy than the base metal. should be filled with weld metal of the same tensile strength as the base metal. should be filled with weld metal of a higher tensile strength than the base metal. can be left unfilled provided adequate wall thickness remains and edges are blended.
Stairway treads that have been worn smooth: a) b) c) d) can be roughened by placing weld beads on the worn surface. should always be replaced. are acceptable provided the tread thickness is adequate. should be repaired with epoxy based materials.